High-temperature ferroelastic phase transition in a perovskite-like complex: [Et4N]2[PbBr3]2
Huang, Yuan; Yang, Jie; Li, Zi-jian; Qian, Kun; Sao, Feng; RSC Advances 9 (2019) 10364–; doi:10.1039/C9RA00804G

data_7232564
_publ_section_title
;
 High-temperature ferroelastic phase transition in a perovskite-like
 complex: [Et4N]2[PbBr3]2
;
_journal_issue                   18
_journal_name_full               'RSC Advances'
_journal_page_first              10364
_journal_paper_doi               10.1039/C9RA00804G
_journal_volume                  9
_journal_year                    2019
_chemical_formula_sum            'C8 H20 Br3 N Pb'
_chemical_formula_weight         577.17
_space_group_crystal_system      hexagonal
_space_group_IT_number           194
_space_group_name_Hall           '-P 6c 2c'
_space_group_name_H-M_alt        'P 63/m m c'
_symmetry_space_group_name_Hall  '-P 6c 2c'
_symmetry_space_group_name_H-M   'P 63/m m c'
_atom_sites_solution_hydrogens   geom
_audit_creation_method           SHELXL-2016/6
_audit_update_record
;
2018-12-08 deposited with the CCDC.    2019-03-26 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            2
_cell_length_a                   10.5952(6)
_cell_length_b                   10.5952(6)
_cell_length_c                   7.9539(6)
_cell_measurement_reflns_used    548
_cell_measurement_temperature    393(2)
_cell_measurement_theta_max      53.2600
_cell_measurement_theta_min      7.3600
_cell_volume                     773.27(9)
_computing_cell_refinement       'Bruker FRAMBO'
_computing_data_collection       'Bruker FRAMBO'
_computing_data_reduction        'Bruker SAINT'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-2016/6 (Sheldrick, 2016)'
_computing_structure_solution    'Bruker SHELXTL'
_diffrn_ambient_temperature      393(2)
_diffrn_measured_fraction_theta_full 0.997
_diffrn_measured_fraction_theta_max 0.988
_diffrn_measurement_device_type  'multiwire proportional'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_type           CuK\a
_diffrn_radiation_wavelength     1.54178
_diffrn_reflns_av_R_equivalents  0.0948
_diffrn_reflns_av_unetI/netI     0.0417
_diffrn_reflns_Laue_measured_fraction_full 0.997
_diffrn_reflns_Laue_measured_fraction_max 0.988
_diffrn_reflns_limit_h_max       12
_diffrn_reflns_limit_h_min       -8
_diffrn_reflns_limit_k_max       12
_diffrn_reflns_limit_k_min       -12
_diffrn_reflns_limit_l_max       5
_diffrn_reflns_limit_l_min       -9
_diffrn_reflns_number            2149
_diffrn_reflns_point_group_measured_fraction_full 0.997
_diffrn_reflns_point_group_measured_fraction_max 0.988
_diffrn_reflns_theta_full        67.679
_diffrn_reflns_theta_max         72.044
_diffrn_reflns_theta_min         4.819
_diffrn_source                   'sealed tube'
_exptl_absorpt_coefficient_mu    30.030
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_correction_T_min  0.04127
_exptl_absorpt_correction_type   multi-scan
_exptl_crystal_colour            colourless
_exptl_crystal_density_diffrn    2.479
_exptl_crystal_description       strip
_exptl_crystal_F_000             524
_exptl_crystal_size_max          0.15
_exptl_crystal_size_mid          0.12
_exptl_crystal_size_min          0.06
_refine_diff_density_max         1.589
_refine_diff_density_min         -0.785
_refine_diff_density_rms         0.192
_refine_ls_extinction_coef       0.0009(3)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     'SHELXL-2016/6 (Sheldrick 2016)'
_refine_ls_goodness_of_fit_ref   1.089
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     89
_refine_ls_number_reflns         316
_refine_ls_number_restraints     129
_refine_ls_restrained_S_all      1.180
_refine_ls_R_factor_all          0.0826
_refine_ls_R_factor_gt           0.0684
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+20.0000P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1252
_refine_ls_wR_factor_ref         0.1358
_reflns_Friedel_coverage         0.000
_reflns_number_gt                224
_reflns_number_total             316
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            c9ra00804g2.cif
_cod_data_source_block           x
_cod_original_cell_volume        773.27(11)
_cod_database_code               7232564
_shelx_shelxl_version_number     2016/6
_shelx_res_checksum              9062